LMucko/crystallography-open-database huggingface dataset:
The crystal structure of Pu3 Co
Larson, A.C.; Cromer, D.T.; Roof, R.B.jr.; Acta Crystallographica (1,1948-23,1967) 16 (1963) 835–836; doi:

data_2310303
_publ_section_title
;
 The crystal structure of Pu3 Co
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              835
_journal_page_last               836
_journal_volume                  16
_journal_year                    1963
_chemical_formula_sum            'Co Pu3'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   3.475
_cell_length_b                   10.976
_cell_length_c                   9.22
_cell_volume                     351.666
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Larson_ACCRA9_1963_1194.cif
_cod_data_source_block           Co1Pu3
_cod_original_cell_volume        351.6656
_cod_original_formula_sum        'Co1 Pu3'
_cod_database_code               2310303
The crystal structure of phase C in the ternary system Ce-Pu-Co
Larson, A.C.; Roof, R.B.jr.; Cromer, D.T.; Acta Crystallographica (1,1948-23,1967) 17 (1964) 1382–1386; doi:

data_2310304
_publ_section_title
;
 The crystal structure of phase C in the ternary system Ce-Pu-Co
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              1382
_journal_page_last               1386
_journal_volume                  17
_journal_year                    1964
_chemical_formula_sum            'Ce Co3 Pu4'
_space_group_IT_number           140
_symmetry_space_group_name_Hall  '-I 4 2c'
_symmetry_space_group_name_H-M   'I 4/m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.73
_cell_length_b                   10.73
_cell_length_c                   5.383
_cell_volume                     619.760
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Larson_ACCRA9_1964_746.cif
_cod_data_source_block           Ce1Co3Pu4
_cod_original_cell_volume        619.7603
_cod_original_formula_sum        'Ce1 Co3 Pu4'
_cod_database_code               2310304
Crystal structure of trifluoro-oxosulphur(VI) hexafluoroarsenate(V), (O S F3)(+) (As F6)(-)
Lau, C.; Lynton, H.; Passmore, J.; Siew, P.Y.; Journal of the Chemical Society. Dalton Transactions, Inorganic Chemistry (1972-) 1973 (1973) 2535–2538; doi:

data_4031202
_publ_section_title
;
 Crystal structure of trifluoro-oxosulphur(VI) hexafluoroarsenate(V), (O S
 F3)(+) (As F6)(-)
;
_journal_name_full
;
Journal of the Chemical Society. Dalton Transactions, Inorganic Chemistry 
(1972-)
;
_journal_page_first              2535
_journal_page_last               2538
_journal_volume                  1973
_journal_year                    1973
_chemical_formula_sum            'As F9 O S'
_chemical_name_systematic        'O S F3 As F6'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.88
_cell_length_b                   7.366
_cell_length_c                   8.473
_cell_volume                     679.044
_citation_journal_id_ASTM        JCDTBI
_cod_data_source_file            Lau_JCDTBI_1973_630.cif
_cod_data_source_block           As1F9O1S1
_cod_original_cell_volume        679.0438
_cod_original_formula_sum        'As1 F9 O1 S1'
_cod_database_code               4031202
Die Kristallstrukturen von Sc Hg, Sc Hg3, Y Cd, Y Hg und Y Hg3
Laube, A.; Nowotny, H.; Monatshefte fuer Chemie (-108,1977) 94 (1963) 851–858; doi:

data_1524798
_publ_section_title
;
 Die Kristallstrukturen von Sc Hg, Sc Hg3, Y Cd, Y Hg und Y Hg3
;
_journal_name_full               'Monatshefte fuer Chemie (-108,1977)'
_journal_page_first              851
_journal_page_last               858
_journal_volume                  94
_journal_year                    1963
_chemical_formula_sum            'Cd Y'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.719
_cell_length_b                   3.719
_cell_length_c                   3.719
_cell_volume                     51.437
_citation_journal_id_ASTM        MOCHAP
_cod_data_source_file            Laube_MOCHAP_1963_715.cif
_cod_data_source_block           Cd1Y1
_cod_original_cell_volume        51.43735
_cod_original_formula_sum        'Cd1 Y1'
_cod_database_code               1524798
Une nouvelle structure ordonnee derivee de la fluorine: Pb3 Zr F10
Laval, J.P.; Frit, B.; Materials Research Bulletin 14 (1979) 1517–1524; doi:

data_1524799
_publ_section_title
;
 Une nouvelle structure ordonnee derivee de la fluorine: Pb3 Zr F10
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              1517
_journal_page_last               1524
_journal_volume                  14
_journal_year                    1979
_chemical_formula_sum            'F10 Pb3 Zr'
_chemical_name_systematic        'Pb3 Zr F10'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.713
_cell_length_b                   12.817
_cell_length_c                   5.909
_cell_volume                     811.356
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            Laval_MRBUAC_1979_409.cif
_cod_data_source_block           F10Pb3Zr1
_cod_original_cell_volume        811.3561
_cod_original_formula_sum        'F10 Pb3 Zr1'
_cod_database_code               1524799
Ueber einige neue Vertreter des Ni As-Typs und ihre kristallchemische Bedeutung
Laves, F.; Wallbaum, H.J.; Zeitschrift fuer Angewandte Mineralogie 4 (1942) 17–46; doi:

data_1524800
_publ_section_title
;
 Ueber einige neue Vertreter des Ni As-Typs und ihre kristallchemische
 Bedeutung
;
_journal_name_full               'Zeitschrift fuer Angewandte Mineralogie'
_journal_page_first              17
_journal_page_last               46
_journal_volume                  4
_journal_year                    1942
_chemical_formula_sum            'Cu1.74 In0.96'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   4.269
_cell_length_b                   4.269
_cell_length_c                   5.239
_cell_volume                     82.686
_citation_journal_id_ASTM        ZANMA4
_cod_data_source_file            Laves_ZANMA4_1942_1500.cif
_cod_data_source_block           Cu1.74In0.96
_cod_original_cell_volume        82.68587
_cod_database_code               1524800
Ueber einige neue Vertereter des NiAs-Typs und ihre kristallchemische Bedeutung
Laves, F.; Wallbaum, H.J.; Zeitschrift fuer Angewandte Mineralogie 4 (1942) 17–46; doi:

data_1524801
_publ_section_title
;
 Ueber einige neue Vertereter des NiAs-Typs und ihre kristallchemische
 Bedeutung
;
_journal_name_full               'Zeitschrift fuer Angewandte Mineralogie'
_journal_page_first              17
_journal_page_last               46
_journal_volume                  4
_journal_year                    1942
_chemical_formula_sum            'Fe1.715 Ge0.975'
_chemical_name_systematic        'Fe2 Ge'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   4.031
_cell_length_b                   4.031
_cell_length_c                   5.022
_cell_volume                     70.670
_citation_journal_id_ASTM        ZANMA4
_cod_data_source_file            Laves_ZANMA4_1942_42.cif
_cod_data_source_block           Fe1.715Ge0.975
_cod_original_cell_volume        70.66965
_cod_database_code               1524801
Structural characteristics of K5 Y (Mo O4)4-alpha crystals
Lazoryak, B.I.; Efremov, V.A.; Kristallografiya 26 (1981) 464–472; doi:

data_1524802
_publ_section_title
;
 Structural characteristics of K5 Y (Mo O4)4-alpha crystals
;
_journal_name_full               Kristallografiya
_journal_page_first              464
_journal_page_last               472
_journal_volume                  26
_journal_year                    1981
_chemical_formula_sum            'K7.5003 Mo2.0001 O24.0003 Y1.5'
_chemical_name_systematic        '(K5 Y (Mo O4)4)1.5'
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   6.035
_cell_length_b                   6.035
_cell_length_c                   20.52
_cell_volume                     647.236
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Lazoryak_KRISAJ_1981_12.cif
_cod_data_source_block           K7.5003Mo2.0001O24.0003Y1.5
_cod_original_cell_volume        647.2358
_cod_database_code               1524802
Magnetic structures of cubic Fe Ge studied by small-angle neutron scatttering
Lebech, B.; Bernhard, J.; Freltoft, T.; Journal of Physics: Condensed Matter 1 (1989) 6105–6122; doi:

data_1524803
_publ_section_title
;
 Magnetic structures of cubic Fe Ge studied by small-angle neutron
 scatttering
;
_journal_name_full               'Journal of Physics: Condensed Matter'
_journal_page_first              6105
_journal_page_last               6122
_journal_volume                  1
_journal_year                    1989
_chemical_formula_sum            'Fe Ge'
_space_group_IT_number           198
_symmetry_space_group_name_Hall  'P 2ac 2ab 3'
_symmetry_space_group_name_H-M   'P 21 3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.689
_cell_length_b                   4.689
_cell_length_c                   4.689
_cell_volume                     103.096
_citation_journal_id_ASTM        JCOMEL
_cod_data_source_file            Lebech_JCOMEL_1989_1944.cif
_cod_data_source_block           Fe1Ge1
_cod_original_cell_volume        103.0957
_cod_original_formula_sum        'Fe1 Ge1'
_cod_database_code               1524803
The lattice spacings of binary tin-rich alloys
Lee, J.A.; Raynor, G.V.; Proceedings of the Physical Society, London 67 (1954) 737–747; doi:

data_1524804
_publ_section_title
;
 The lattice spacings of binary tin-rich alloys
;
_journal_name_full               'Proceedings of the Physical Society, London'
_journal_page_first              737
_journal_page_last               747
_journal_volume                  67
_journal_year                    1954
_chemical_formula_sum            'Cd0.01 Sn0.99'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  'I 4bw 2bw -1bw'
_symmetry_space_group_name_H-M   'I 41/a m d :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.83
_cell_length_b                   5.83
_cell_length_c                   3.18
_cell_volume                     108.085
_citation_journal_id_ASTM        PPSOAU
_cod_data_source_file            Lee_PPSOAU_1954_727.cif
_cod_data_source_block           Cd0.01Sn0.99
_cod_original_cell_volume        108.0847
_cod_original_sg_symbol_Hall     '-I 4bd 2 (x+1/2,y+1/4,z+1/8)'
_cod_database_code               1524804
Solid state properties of group IVb carbonitrides
Lengauer, W.; Binder, S.; Aigner, K.; Groboth, G.; Guillou, A.; Ettmayer, P.; Debuigne, J.; Journal of Alloys Compd. 217 (1995) 137–147; doi:

data_1524805
_publ_section_title
;
 Solid state properties of group IVb carbonitrides
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              137
_journal_page_last               147
_journal_volume                  217
_journal_year                    1995
_chemical_formula_sum            'C N Zr2'
_chemical_name_systematic        'Zr3 C N'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.636
_cell_length_b                   4.636
_cell_length_c                   4.636
_cell_volume                     99.639
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Lengauer_JALCEU_1995_68.cif
_cod_data_source_block           C1N1Zr2
_cod_original_cell_volume        99.63922
_cod_original_formula_sum        'C1 N1 Zr2'
_cod_database_code               1524805
Kristallstruktur von Cu10 Sn3 (m)
Lenz, J.; Schubert, K.; Monatshefte fuer Chemie (-108,1977) 102 (1971) 1689–1698; doi:

data_1524806
_publ_section_title
;
 Kristallstruktur von Cu10 Sn3 (m)
;
_journal_name_full               'Monatshefte fuer Chemie (-108,1977)'
_journal_page_first              1689
_journal_page_last               1698
_journal_volume                  102
_journal_year                    1971
_chemical_formula_sum            'Cu10 Sn3'
_space_group_IT_number           176
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   7.313
_cell_length_b                   7.313
_cell_length_c                   7.87
_cell_volume                     364.499
_citation_journal_id_ASTM        MOCHAP
_cod_data_source_file            Lenz_MOCHAP_1971_1616.cif
_cod_data_source_block           Cu10Sn3
_cod_original_cell_volume        364.4991
_cod_database_code               1524806
Ueber einige Leerstellen- und Stapelvarianten der beta-Messing Strukturfamilie
Lenz, J.; Schubert, K.; Zeitschrift fuer Metallkunde 62 (1971) 810–816; doi:

data_1524807
_publ_section_title
;
 Ueber einige Leerstellen- und Stapelvarianten der beta-Messing
 Strukturfamilie
;
_journal_name_full               'Zeitschrift fuer Metallkunde'
_journal_page_first              810
_journal_page_last               816
_journal_volume                  62
_journal_year                    1971
_chemical_formula_sum            'Cu0.7 Zn2'
_space_group_IT_number           174
_symmetry_space_group_name_Hall  'P -6'
_symmetry_space_group_name_H-M   'P -6'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   4.275
_cell_length_b                   4.275
_cell_length_c                   2.59
_cell_volume                     40.992
_citation_journal_id_ASTM        ZEMTAE
_cod_data_source_file            Lenz_ZEMTAE_1971_1653.cif
_cod_data_source_block           Cu0.7Zn2
_cod_original_cell_volume        40.99233
_cod_database_code               1524807
Comparative investigation of structural transport properties of L10 Ni Pt and Co Pt phases; the role of magnetism
Leroux, C.; Cadeville, M.C.; Pierron-Bohnes, V.; Inden, G.; Hinz, F.; Journal of Physics F 18 (1988) 2033–2051; doi:

data_1524808
_publ_section_title
;
 Comparative investigation of structural transport properties of L10 Ni Pt
 and Co Pt phases; the role of magnetism
;
_journal_name_full               'Journal of Physics F'
_journal_page_first              2033
_journal_page_last               2051
_journal_volume                  18
_journal_year                    1988
_chemical_formula_sum            'Co0.5 Pt0.5'
_chemical_name_systematic        '(Co0.5 Pt0.5)'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   3.835
_cell_length_b                   3.835
_cell_length_c                   3.835
_cell_volume                     56.402
_citation_journal_id_ASTM        JPFMAT
_cod_data_source_file            Leroux_JPFMAT_1988_1187.cif
_cod_data_source_block           Co0.5Pt0.5
_cod_original_cell_volume        56.40221
_cod_database_code               1524808
The crystal structure, thermal behaviour and IR spectrum of copper tetraammine dithionate
Leskelae, M.; Valkonen, J.; Hoppe, R.; Acta Chemica Scandinavica, Series A: (28,1974-) 32 (1978) 805–809; doi:

data_1524809
_publ_section_title
;
 The crystal structure, thermal behaviour and IR spectrum of copper
 tetraammine dithionate
;
_journal_name_full
'Acta Chemica Scandinavica, Series A: (28,1974-)'
_journal_page_first              805
_journal_page_last               809
_journal_volume                  32
_journal_year                    1978
_chemical_formula_sum            'Cu H12 N4 O6 S2'
_chemical_name_systematic        '(Cu (N H3)4) (S2 O6)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 145.12
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.148
_cell_length_b                   10.604
_cell_length_c                   11.675
_cell_volume                     506.058
_citation_journal_id_ASTM        ACAPCT
_cod_data_source_file            Leskelae_ACAPCT_1978_420.cif
_cod_data_source_block           H12Cu1N4O6S2
_cod_original_cell_volume        506.0583
_cod_original_formula_sum        'H12 Cu1 N4 O6 S2'
_cod_database_code               1524809
Exchange interactions in polynuclear transition metal complexes. Structural properties of cesium tribromocuprate(II), Cs Cu Br3, a strongly coupled copper(II) system
Li, T.I.; Stucky, G.D.; Inorganic Chemistry 12 (1973) 441–445; doi:

data_4343671
_publ_section_title
;
 Exchange interactions in polynuclear transition metal complexes.
 Structural properties of cesium tribromocuprate(II), Cs Cu Br3, a
 strongly coupled copper(II) system
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              441
_journal_page_last               445
_journal_volume                  12
_journal_year                    1973
_chemical_formula_sum            'Br3 Cs Cu'
_chemical_name_systematic        'Cs Cu Br3'
_space_group_IT_number           20
_symmetry_space_group_name_Hall  'C 2c 2'
_symmetry_space_group_name_H-M   'C 2 2 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.776
_cell_length_b                   7.666
_cell_length_c                   12.653
_cell_volume                     1239.245
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Li_INOCAJ_1973_623.cif
_cod_data_source_block           Br3Cs1Cu1
_cod_original_formula_sum        'Br3 Cs1 Cu1'
_cod_database_code               4343671
Exchange interactions in polynuclear transition metal complexes. Structural properties of cesium tribromocuprate(II), Cs Cu Br3, a strongly coupled copper(II) system
Li, T.I.; Stucky, G.D.; Inorganic Chemistry 12 (1973) 441–445; doi:

data_4343672
_publ_section_title
;
 Exchange interactions in polynuclear transition metal complexes.
 Structural properties of cesium tribromocuprate(II), Cs Cu Br3, a
 strongly coupled copper(II) system
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              441
_journal_page_last               445
_journal_volume                  12
_journal_year                    1973
_chemical_formula_sum            'Br4 Cs2 Cu'
_chemical_name_systematic        'Cs2 Cu Br4'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.168
_cell_length_b                   7.954
_cell_length_c                   12.914
_cell_volume                     1044.436
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Li_INOCAJ_1973_624.cif
_cod_data_source_block           Br4Cs2Cu1
_cod_original_formula_sum        'Br4 Cs2 Cu1'
_cod_database_code               4343672
Darstellung, Eigenschaften und Kristallstruktur von Rhenium(VII)-nitridchlorid, Re N Cl4
Liese, W.; Walker, I.; Dehnicke, K.; Straehle, J.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (33,1978-41,1986) 34 (1979) 693–696; doi:

data_7221223
_publ_section_title
;
 Darstellung, Eigenschaften und Kristallstruktur von
 Rhenium(VII)-nitridchlorid, Re N Cl4
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (33,1978-41,1986)
;
_journal_page_first              693
_journal_page_last               696
_journal_volume                  34
_journal_year                    1979
_chemical_formula_sum            'Cl4 N Re'
_chemical_name_systematic        'Re N Cl4'
_space_group_IT_number           1
_symmetry_space_group_name_Hall  'P 1'
_symmetry_space_group_name_H-M   'P 1'
_cell_angle_alpha                90.09
_cell_angle_beta                 90.17
_cell_angle_gamma                89.88
_cell_formula_units_Z            2
_cell_length_a                   8.278
_cell_length_b                   8.281
_cell_length_c                   4.057
_cell_volume                     278.106
_citation_journal_id_ASTM        ZNBAD2
_cod_data_source_file            Liese_ZNBAD2_1979_575.cif
_cod_data_source_block           Cl4N1Re1
_cod_original_cell_volume        278.1057
_cod_original_sg_symbol_Hall
;
P 1 (-1/2*x+1/2*y+1/2*z,1/2*x-1/2*y+1/2*z,1/2*x+1/2*y-1/2*z)
;
_cod_original_formula_sum        'Cl4 N1 Re1'
_cod_database_code               7221223
Untersuchungen in den ternaeren Systemen Mg-Cu-Zn, Mg-Ni-Zn und Mg-Cu-Ni
Lieser, K.H.; Witte, H.; Zeitschrift fuer Metallkunde 43 (1952) 396–401; doi:

data_1524810
_publ_section_title
;
 Untersuchungen in den ternaeren Systemen Mg-Cu-Zn, Mg-Ni-Zn und Mg-Cu-Ni
;
_journal_name_full               'Zeitschrift fuer Metallkunde'
_journal_page_first              396
_journal_page_last               401
_journal_volume                  43
_journal_year                    1952
_chemical_formula_sum            'Cu2 Mg'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   7.021
_cell_length_b                   7.021
_cell_length_c                   7.021
_cell_volume                     346.096
_citation_journal_id_ASTM        ZEMTAE
_cod_data_source_file            Lieser_ZEMTAE_1952_1563.cif
_cod_data_source_block           Cu2Mg1
_cod_original_cell_volume        346.0963
_cod_original_formula_sum        'Cu2 Mg1'
_cod_database_code               1524810